Publisher’s version / Version de l'éditeur:
Applied Scientific Research, 26, pp. 86-92, 1972-09-01
READ THESE TERMS AND CONDITIONS CAREFULLY BEFORE USING THIS WEBSITE. https://nrc-publications.canada.ca/eng/copyright
Vous avez des questions? Nous pouvons vous aider. Pour communiquer directement avec un auteur, consultez la
première page de la revue dans laquelle son article a été publié afin de trouver ses coordonnées. Si vous n’arrivez pas à les repérer, communiquez avec nous à PublicationsArchive-ArchivesPublications@nrc-cnrc.gc.ca.
Questions? Contact the NRC Publications Archive team at
PublicationsArchive-ArchivesPublications@nrc-cnrc.gc.ca. If you wish to email the authors directly, please see the first page of the publication for their contact information.
NRC Publications Archive
Archives des publications du CNRC
This publication could be one of several versions: author’s original, accepted manuscript or the publisher’s version. / La version de cette publication peut être l’une des suivantes : la version prépublication de l’auteur, la version acceptée du manuscrit ou la version de l’éditeur.
Access and use of this website and the material on it are subject to the Terms and Conditions set forth at
The activation volume associated with the plastic deformation of ice
Krausz, A. S.
L’accès à ce site Web et l’utilisation de son contenu sont assujettis aux conditions présentées dans le site LISEZ CES CONDITIONS ATTENTIVEMENT AVANT D’UTILISER CE SITE WEB.
NRC Publications Record / Notice d'Archives des publications de CNRC:
Appl. Sci. Res. 26 May 1972
T H E ACTIVATION VOLUME ASSOCIATED W I T H
T H E PLASTIC DEFORMATION O F ICE
Dept. of Mech. Eng. University of Ottawa, Ottawa, CANADA
Stress relaxation experiments are carried out on single, bi, tri and quadri crystals of ice t o obtain information on the rate controlling process. The results are analyzed with the rate theory developed previously. The study indicated that the energy barrier is asymmetrical and that the rate con- trolling process is associated with the Peierls barrier, with the dislocation intersection mechanism, or with the non-conservative motion of jogs. It seems unlikely that climb would control the dislocation motion in ice.
§ 1. Introduction
I t has been observed both in nature and under laboratory con- ditions that, as water freezes, ice tubes and needles occasionally grow from the frozen surface. The growth mechailism has been investigated in detail and reported [I]. I n the course of the growth study, it was realized that these tubes and needles offer particularly suitable specimens for the investigation of some of the physical properties associated with single, bi, tri and quadri crystals. The plastic deformation of the needles is of special interest because they are grown without being subjected to any mechanical effect, a condition seldom achieved for ice with the conventional methods of bi, tri and quadri crystal growth. The availability of good bi, tri and quadri crystals together with the lack of information on their plastic behavior made a study of the associated thermally activated process a timely project. The results of this investigation are now reported.
* Formerly Research Officer, Geotechnical Section, Division of Building Research, National Research Council of Canada, Ottawa.
PLASTIC DEFORAIATION OF ICE 87
3 2. Experimental procedure
Ice needles, about 50 mnl in length and 1.5 to 2 nlm in diameter, were grown with the technique reportecl previously [I]. In all of the sevellteell specimens that were tested, the grain boundaries were straight and pal-allel to the specimen axis over the whole length of the crystals. The angle between the C-axis and the specimen axis vai-iecl from 25 degrees to 70 degrees.
Sti-ess relaxation tests were carried out in tension a t several strain levels on a Tinius-Olsen U-Celtronic testing machine. The specimen was frozen into two metal gi-ips and kept a t 263°K 0.2"I< in a cold chamber. The chamber was cooled with four IFB-32-015-G1 Frigistor solid state heat pumps controlled with a simple on-off circuit using a YSI No. 44002 precision thermistor. To facilitate the analysis, the measurements were made until no further load change hacl occurred.
Strain rate change expcrime~lts as well as creep tests both in tension and in bending were also cai-ried out. Only the stress relaxation results were used for the detailed analysis of the rate- controlling mechanism because, for ice, the transition effects are very pronounced in the strain rate change ancl creep tests. I t call be noted, nevertheless, that both of these sets of observations support the coilclusions clerivecl from the stress relaxation studies.
§ 3. Discussion
The experimental results were analyzecl with the theory developed in a series of recent investigations [2, 31. These studies inclicated that the thermally activated dislocation movement in ionic and covalent ci-ystals call be clescribed with a linearly stress depenclent apparent activation energy and that the rate-controlling mecha- nism is associatecl with an asymmetrical energy barrier. Using the absolute sate theory, it was shown that the stress dependence of the dislocation velocity can be expressed as [2, 4-61
The subscripts f and b indicate respectively that the quantity is associated with the forward or backward movement of the dis- location, V is the activation volume, T e f f is the effective stress acting
on the dislocation, K is the transmission coefficient, I is the average
distance travelled by the dislocation after each activation, Q , and
are the partition functions of the initial and activated state re- spectively, AE is the activation energy; the other symbols have their usual meaning.
The relationship between the dislocation velocity and the stress rate measured in stress relaxation can be derived from Orowan's equation 
j = ~ ~ P V ( T ~ P P )
where j is the strain rate, a is a geometrical factor,
ZIis the Burgers vector and p is the mobile dislocation density. In stress relaxation
where 1 is the composite elastic modulus of the specimen and testing apparatus [ 8 ] . Hence,
Combining (2) with (1) the stress relaxation can be described as
- - 1olbpA
;exp ---- T ' f ~ e f f
Iexp - V b ~ e f f
k T Iz T
- - A f exp --- V f ~ e f f -- V b ~ e f f
Because (1) was derived for ionic and covalent crystals, it is reason- able to expect that the plastic deformation of ice is controlled by a similar thermally activated process. Using this assumption, the stress relaxation in ice could be analyzed in terms of physical quantities using (3).
It was found that (3) described well the experimental observations for all of the crystals. A typical example is shown in Fig. 1. This result is important because the agreement indicates that the mecha- nism of plastic deformation of ice is associated with an asymmetrical
P L A S T I C D E F O R M A T I O N O F I C E 89
i l i Y i ; i I
Fig. 1. A typical stress relaxation rexult. The syn~bols represent the cx- periinental values, the curve was calculatccl with (3). No effort was nlaclc to
obtain the best fit. The activation parameters are,
A D = 0.015 lcg mm-%min-I
triangular energy barrier ancl justifies the assumption macle in using (3).
In stress relaxation studies, the change of the effective stress Teff
is often represented in function of the logarithm of time t. I t is useful, therefore, t o illustrate the stress relaxation behavior of ice obtained in the present investigation in this coordinate system as well. An example is shown in Fig. 2.
The good agreement obtained between the theory and the ex- perimental results supports the use of (3) for the evaluation of the activation volume. The analysis shows that the activation volume in the forward direction is
r , - , 7,: >
I;ig. 2. -4 typical strcss relaxation rcsult in wllicll the strcss clla~lge is plotted in function of ihc logarithm of time. The sy~llbols represent the experinlental vslucs and the curve was calculated fro111 (3) by numerical integration.
The activation parameters are,
Thcse activation volunlcs indicate t h a t the rate-controlling mecha- nism in ice may be one of the following:
1. Peierls barrier
2. clislocation intersection, or 3. nonconsei-vative motion of jogs.
I t is unliltely t h a t clislocation climb ~vould have any effect on the plastic clcformation of ice single, bi, tri and quadri crystals. This conclusion confirms the results obtained in previous studies carried out on polycrystalline ice  and on ice single crystals [lo]. For all of the investigated single, bi, tri ancl quadri crystals, the defor- mation behavior and the activation parameters were similar indi- cating t h a t the rate-controlling process is not affected by the grain boundaries. The usually observed difference in the stress exponents of single and polycrystalline ice is, therefore, due to the internal strcss and not t o a difference in the rate-controlling mechanism.
PLASTIC DEFORhIATION O F ICE 9 1
I;ig. 3. Icc necclle bent into a loop in about one minutc a t - 10°C.
I t is of interest to nle~ltion a rather stril<ing observatioil illacle cluriilg the bending tests. The investigated small diameter crystals coulcl be bent readily into a full loop over a periocl of time as short as 1 minute (Fig. 3). The crystals clicl not break during this severe clefor- maiion but, occasionally, separation along the grain bouilclary did occur. I t was usually possible to straighten the crystals after bending.
The author wishes to thank 13. Harron for his contributions to the the experiments and
M.Zulter for assistance in the analysis of the
experimental results. This is a contribution from the Divisioil of Builcling Research, National Research Council of Canada and is published with the approval of the Director of the division.
92 PLASTIC DEFORMLIATION O F ICE
R E F E R E N C E S
[I] I<RAUSZ, A. S., U. I-IARRON a n d G. G. LITVAN, Nature 215 (1967) 271.  I<RAUSZ, A. S., Acta Met. 16 (1968) 897.
 I<RAUSZ, -4. S., hfater. Sci. and Eng. 4 (1969) 193.
 GLASSTONE, S., I<. J. L A I D L E R , a n d I-I. E Y R I K G , T h c Thcory of Rate Processes, RIcGram-Hill, New York (1940).
 LAIDLER, I<. J., Chcnlical Kinetics, AIcGraw-I-Iill, New York (1965).
 E Y R ~ N G , M., Energetics 3, Science Publishers Inc., Gordon a n d Breach N.Y. (1967) 3.  ORO!VAN, E., ~ ' T O C . P l l y ~ . SOC. 52 (1940) 8.
 Guru, F., and P. L. PRATT, P h y s S t a t . Sol. 6 (1964) 1 1 I.  IiRnusz, .4. S., Scripta Met. 2 (1968) 615.